Advances in Condensed Matter Physics

Volume 2013 (2013), Article ID 104806, 13 pages

http://dx.doi.org/10.1155/2013/104806

## Understanding Multiferroic Hexagonal Manganites by Static and Ultrafast Optical Spectroscopy

^{1}Department of Electrophysics, National Chiao Tung University, Hsinchu 30010, Taiwan^{2}Advanced Ultrafast Laser Research Center, University of Electro-Communications, Chofugaoka 1-5-1, Chofu, Tokyo 182-8585, Japan

Received 25 June 2012; Revised 19 January 2013; Accepted 28 January 2013

Academic Editor: R. N. P. Choudhary

Copyright © 2013 Yu Ting Wang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

Multiferroic hexagonal manganites ReMnO_{3} studied by optics are reviewed. Their electronic structures were revealed by static linear and nonlinear spectra. Two transitions located at 1.7 eV and 2.3 eV have been observed and attributed to the interband transitions from the lower-lying Mn^{3+} and states to the Mn^{3+} state, respectively. These so-called d-d transitions exhibit a blueshift as decreasing temperatures and an extra blueshift near . This dramatic change indicates that the magnetic ordering seriously influences the electronic structure. On the other hand, the ultrafast optical pump-probe spectroscopy has provided the important information on spin-charge coupling and spin-lattice coupling. Because of the strongly correlation between electronic structure and magnetic ordering, the amplitude of the initial rising component in shows striking changes at the vicinity of . Moreover, the coherent optical and acoustic phonons were observed on optical pump-probe spectroscopy. Both the amplitude and dephasing time of coherent phonons also exhibit significant changes at , which provide the evidence for spin-lattice interaction in these intriguing materials.

#### 1. Introduction

Multiferroic materials [1–4] with the coexistence of various ferroic order (ferromagnetic, ferroelectric, or ferroelastic) have attracted great attention in condensed matter research due to their great potential for applications in the fields of oxide electronics, spintronics, and even the green energy devices for reducing the power consumption. With multiferroic oxides (in single phase), the coupling interaction among various order parameters causes the so-called magnetoelectric effect [5–10]. In this, a polarization can be induced by applying a magnetic field or a magnetization can be induced by applying an electric field. Although the properties of electricity and magnetism were combined into one common discipline by the Maxwell equations, the electric and magnetic orderings in solid-state materials are always considered separately. This is because that the electric charges of electrons and ions are responsible for the charge effects, whereas the electron spins govern the magnetic properties.

Prellier et al. [11] classified the characteristics of multiferroic materials into three categories. The first is Bi-based compounds, such as BiMnO_{3} and BiFeO_{3}. The second is perovskites and related ReMnO_{3} compounds (Re = Y, Ho, Er, Tm, Yb, and Lu). The third is ReMn_{2}O_{5} (Re is rare earth element). Additionally, Cheong and Mostovoy [12] summarized the classification of ferroelectrics into “proper” and “improper” according to their mechanisms of inversion symmetry breaking. In proper ferroelectrics, the main driving force toward the polar state was associated with the electronic pairing. On the other hand, the induced polarization in improper ferroelectrics involves a more complex lattice distortion or other accidental orderings. For example, the hexagonal manganite ReMnO_{3} compounds show a lattice distortion to enlarge their unit cell, which is the so-called geometric ferroelectricity [13–15].

The aim of this paper is to understand the multiferroic hexagonal manganites studied by some optical techniques. In Section 2, the overall features of manganites are introduced. The structure of rare earth manganite is strongly depending on the size of rare earth and also temperature. The environment of Mn ions significantly affects its electronic structure which was investigated by static linear and nonlinear spectra in Section 3. Section 4 is the main part of this paper. The ultrafast spectroscopies demonstrate the interaction between electron, phonon, and spin systems on multiferroic hexagonal manganites. Finally, the summary and future outlook will be given in Section 5.

#### 2. The Characteristics of Multiferroic Manganites ReMnO_{3}

Recently, multiferroic rare earth manganites (ReMnO_{3}) have attracted a great deal of attention due to their manifestations of intriguing and significant couplings between the magnetic and electric order parameters. Generally, ReMnO_{3} has two kinds of multiferroic structures, that is, hexagonal and orthorhombic. The rare earth (Re^{3+}) ionic size shrinks from 1.11 Å to 0.94 Å with decreasing the atomic number and reducing the electrons residing in the 4f orbit, called the lanthanum contraction effect. The rare earth ions (Re^{3+}) have closely chemical properties because the same electronic configurations of 5s^{2}5p^{6} for outermost electrons. The coexistence of ferroic orders in ReMnO_{3} with hexagonal (smaller ionic radius of rare earth Re = Sc, Y, and from Ho to Lu) or orthorhombic (larger ionic radius of rare earth Re = La to Dy) (shown in Figure 1) structure yields complex physics in the intimate interactions among charge, orbital, lattice, and spin degrees of freedom. It also has fascinating physical properties which might lead to promising applications. The orthorhombic structure with a *Pnma* space group forms the stable crystal structure of ReMnO_{3} perovskite oxides with Re = La to Dy, which belongs to the magnetic ferroelectrics induced by magnetic ordering [8, 16]. Furthermore, another family of compounds with smaller ionic size (for Re = Y, Ho, Er, Yb, Lu, etc.) forms the stable hexagonal structure with *cm* space group. The critical point of the structure transition is located near YMnO_{3} (Y^{3+} = 1.06 Å) and HoMnO_{3} (Ho^{3+} = 1.05 Å). Consequently, the crystal structures of these two families have been transformed from hexagonal to orthorhombic (or vice versa) by many experimental techniques, for example, high-temperature and high-pressure processes [17, 18], chemical solution deposition (CSD) [19], the metal-organic chemical vapor deposition (MOCVD) [20], molecular beam epitaxy (MBE) [21], sputtering [22], and pulsed laser deposition (PLD) [16, 23].

In the following, we are going to focus on recent studies on the multiferroic hexagonal manganites (ReMnO_{3}, Re = rare earth) which have properties similar to various rare-earth elements, both electric transportation or magnetic behaviors. For example, the hexagonal HoMnO_{3} has ferroelectric ordering at Curie temperature = 875 K, the antiferroicmagnetic (AFM) Mn^{3+} ordering at Néel temperature = 76 K, and the magnetic Ho^{3+} ordering at = 4.6 K, in which the magnetically active ions are the high spin Mn^{3+} (3d^{4}, *S* = 2) and Ho^{3+} (4f^{10}) [5, 14, 33, 40–45]. The ferroelectricity in magnetoelectric ReMnO_{3} is caused by a buckling of the layered MnO_{5} polyhedral and is accompanied by displacements of the Re ions, which lead to a net electric polarization. In 2004, through X-ray diffraction and first principle density functional calculations, Van Aken et al. [14] demonstrated the previous scenario in the hexagonal manganite YMnO_{3}, as shown in Figure 2 which presents the “geometric” generation of polarization and describes the tilting of a rigid MnO_{5} block with a magnetic Mn atom at the center. The magnetic structure has been studied by various experimental methods, such as neutron diffraction [45, 46] or second harmonic generation (SHG) [33, 47]. In *cm* hexagonal manganites, each Mn^{3+} ion is surrounded by five O^{2-} ions, forming triangular planar sublattices in the basal plane (*a-b* plane). The magnetic order of Mn^{3+} is mainly dominated by AFM in-plane Mn-O-Mn superexchange interaction. Therefore, the triangular lattice of the Mn atoms exhibits strong geometrical frustration effect [48]. Furthermore, when the temperature cools to near , the strong superexchange leads to a 120° arrangement between neighboring Mn^{3+} spins in the basal plane which breaks the triangular frustration. In addition, the spins of Mn rotate with an angle of 90° at (e.g., for *h*-HoMnO_{3}, ~ 33 K) due to the onset of the AFM order of the Re moments, indicating the interaction between Re^{3+} and Mn^{3+} spins. Another magnetic transition at involves the complete magnetic order of the Re^{3+} ions (e.g., for *h*-HoMnO_{3}, ~ 5 K).

In addition, there are many studies showing the anomaly around , such as the dielectric constant [49], specific heat measurements [50], and the lattice constant measurements [51], which are attributed to the indirect coupling via lattice strain (spin-lattice coupling). Recently, Lee et al. [52] observed the giant magnetoelastic effect in hexagonal YMnO_{3} and LuMnO_{3} by using the high-resolution neutron and synchrotron powder diffraction experiments. They further claimed that the magnetoelectric (ME) coupling can be interpreted by the giant magnetoelastic effect very well in ReMnO_{3}, that is, the magnetic long-range ordering induced the very large displacements of all atoms at . In other words, the magnetoelastic coupling allowed the atoms to undergo an isostructural transition, which has been regarded as the primary source of the magnetoelectric phenomena. In hexagonal ReMnO_{3}, this magnetoelastic effect is two orders of magnitude larger than those appearing in other magnetic materials. Therefore, the gigantic magnetoelastic coupling plays a crucial role in dominating many physical properties in hexagonal ReMnO_{3}.

Femtosecond pump-probe spectroscopy has been established as a protocol for studying the interactions between electrons, phonons, and magnons [35, 53–59] and is therefore employed with these multiferroic ReMnO_{3} materials to gain insight into the magnetoelastic effect. By measuring the transient reflectivity () or transmittance (), we can observe the intricate correlation processes among the charge, lattice, and spin degrees of freedom, which are explicitly recognized in different characteristic time scales. Thus, the microscopic mechanism of the magnetoelectric coupling or magnetoelastic behavior in this kind of strongly correlated materials can be revealed.

#### 3. Electronic Structure Revealed by Optical Spectroscopy

To understand the extensive physical properties in multiferroic ReMnO_{3} materials, it is crucial to realize the electronic band structure. With respect to the crystal structure of hexagonal ReMnO_{3} manganites with MnO_{5} bipyramids, in contrast with the MnO_{6} octahedron of orthorhombic structure which split to and , the crystal field symmetry leads the quintet d levels of Mn^{3+} ion splits into two low lying doublets of and (/ and /) states and one singlet () state. In general, optical spectroscopy is one of the powerful tools for investigating the electronic band structure in materials. Therefore, this structural difference between the hexagonal and orthorhombic phases could be disclosed by the optical spectra [60, 61].

##### 3.1. Linear Optical Absorption Spectra

The first optical measurements in hexagonal YMnO_{3} were performed by Kritayakirana et al. in 1969 [62], who observed that a near infrared absorption edge moves to higher energy with lowering temperature. For the case of hexagonal ScMnO_{3} and ErMnO_{3}, the spectra of the real and imaginary parts of the dielectric function were also measured by Kalashnikova and Pisarev [63]. An abnormally drastic absorption peak in the region of 1.57–1.59 eV is the most pronounced feature in the dielectric spectra. This peak exhibits asymmetry and can be decomposed into two components by peak fitting with the Gaussian functions. Furthermore, the absorption intensity in the region above 2.2–2.4 eV increases with photon energy. In addition, hexagonal HoMnO_{3} [64] and LuMnO_{3} [31] also exhibit similar results. It is noteworthy that the near infrared absorption peak exhibits a substantial blueshift of ~0.16 eV from 300 K to 10 K as shown in Figure 3. Recently, Choi et al. [32] reported a systematic study on the hexagonal ReMnO_{3} (R = Gd, Tb, Dy, and Ho), and the overall features in the spectra are similar to previous results. The most surprising part of those results is that the temperature-dependent absorption peak at ~1.7 eV shows an unexpectedly large blueshift near among the rare-earth ions of Re = Lu, Gd, Tb, Dy, and Ho, as shown in Figure 4(a).

The assignment of the optical absorption peak at ~1.7 eV has also been an issue. One interpretation is that it comes from the charge transfer transition from the O 2p to the Mn 3d states [30, 63, 65, 66]. The photoemission spectroscopy (PES) study proposed that the O 2p is the highest occupied state, while the Mn state is mostly unoccupied. Other occupied Mn 3d states (/, and /) lie deep below [65]. The result of the first-principle electronic structure calculations also suggested that the top of the valence band is mainly determined by the O 2p states, and the lowest unoccupied band is formed by the of Mn [30, 66]. The other interpretation, which is also an extensively convincing explanation, is that it comes from on-site d-d transition between the Mn 3d levels [31, 34, 64, 67]. The transition was attributed to the d-d transition between occupied and (/, and /) orbitals and the unoccupied () orbit, as shown in Figure 4(b). Because of the selection rule, transitions between d orbitals are forbidden. However, the selection rule is relaxed through the strong hybridization between the O 2p bands and transition metal d bands, which was observed in the hexagonal phase but not in the orthorhombic phase [60]. Furthermore, the strong peak at ~5 eV is attributed to the charge transfer transition from the hybridized O 2p level to the Mn level.

The other feature of the near infrared absorption peak is that it shows the blueshift as decreasing temperatures accompanying the dramatic changes near , which indicates the effective coupling between the electronic structure and the magnetic ordering. Souchkov et al. [31] attributed this temperature-dependent blueshift to the effects of exchange interactions between the Mn^{3+} ions. The superexchange between Mn^{3+} neighbors leads to lower / levels, whereas the level is rarely affected (see Figure 4(b)). Moreover, together with the temperature-dependent and magnetic-dependent results [32] further implies that the magnetic ordering seriously influences the electronic structure.

##### 3.2. Second Harmonic Generation Spectra

From the linear absorption spectra, the strong absorption caused by the d-d transition from to was clearly observed in hexagonal manganites. But the transition from to is another question. Recently, the second harmonic generation (SHG) was successfully used to explore the hidden localized d-d transitions, even those embedded in the much stronger absorption peaks [68]. The nonlinear polarization induced by optical waves is given by where is the nonlinear polarization induced in a medium. and are the electric field components of the fundamental light. and are the second-order nonlinear susceptibility tensor which are uniquely defined by the crystalline and magnetic structure of the crystal, respectively. The subscripts, , and correspond to the Cartesian coordinate axes , , and . is the direction of the nonlinear polarization generated; and are the directions of applied optical field.

There are two types of optical SHG in multiferroic hexagonal manganites. One is caused by the noncentrosymmetric ferroelectric ordering of charges and the nonlinear susceptibility is time invariant (*i*-type). The other is due to the centrosymmetric antiferromagnetic ordering of spins and the susceptibility is time noninvariant (*c*-type) [34]. Table 1 lists the allowed susceptibility tensor components in *i*-type and *c*-type. Thus, the SHG contribution from ferroelectric and antiferromagnetic can be distinguished easily. Figure 5 summarizes the magnetic symmetries of all the hexagonal ReMnO_{3} compounds as derived from the SHG experiments [33].

The polarization with the space group *cm* below the Curie temperature is
The contribution from antiferromagnetic below for the space group P__6___{3}*c m* (e.g., YMnO

_{3}[68, 69]) is

Figure 6(a) exhibits the SHG spectra of component in YMnO_{3} at 6 K [34]. The strong peak is centered at 2.7 eV, which could be assigned to (corresponds to ) transition. Figure 6(b) right panel shows the spectrum of . Peaks at 2.46 eV represent the (corresponds to ) transition. These assignments have been proved by several studies [47, 68, 69]. In the inset of Figure 6(b), the temperature-dependent intensity of 2.46 eV disappears once the temperature is higher than , which strongly indicates the closed correlation between the antiferromagnetic order parameter and SHG.

Consequently, the electronic structure of hexagonal manganites has been clearly depicted by linear and nonlinear optical spectroscopy, which further provides the basis for the excitation and relaxation of electrons in pump-probe spectroscopy.

#### 4. Ultrafast Pump-Probe Spectroscopy

Ultrafast optical pump-probe spectroscopy has proven to be a powerful tool to investigate the dynamics of electron-electron interaction, electron-phonon interaction, and electron-spin interaction in various materials (see, e.g., [70–72]). To understand the underlying mechanisms in strongly correlated materials, the interactions between these order parameters should be derived first. Because of the different characteristic time scales and characteristic behavior for various degrees of freedom existing in these complex materials, ultrafast spectroscopy can determine the coupling between each order of parameters.

As shown in Figure 7, the general idea of the pump-probe technique is that changes of a sample induced by a pump pulse are obtained by detecting the change in the reflectivity or transmissivity of probe pulses as a function of probe delay time. The femtosecond time evolutions are derived by delaying the relative arrival time between the pump and probe pulses using a mechanical delay line. The fluence of a probe pulse is usually much weaker than that of a pump pulse in order to avoid second excitation in the samples. The polarizations of pump and probe pulses are set perpendicular to avoid interference between pump and probe beams [73].

Generally, this pump-probe spectroscopy composes two kinds of signals of the decay background and the oscillation, which relates to the relaxation of carriers and the dynamics of phonons or spins, respectively. By the Fourier transform, the frequency of phonon modes can be doubly obtained from the oscillation signals in pump-probe spectroscopy. Moreover, the phonon dynamics, that is, the time-evolution of oscillation signals, can be revealed by short-time Fourier transform (STFT), which cannot be reached by common Raman spectroscopy. Thus, the pump-probe spectroscopy is a powerful tool to provide the information in time- and frequency-domain simultaneously.

##### 4.1. Spin-Charge Coupling

Since the magnetic ordering and the electronic structure of manganites are strongly correlated, as found in temperature-dependent absorption spectra, there is a strong coupling between charge and spin, which can be revealed by the time-resolved femtosecond spectroscopy [72]. Shih et al. observed the spin-charge coupling by various photon energy excitations on hexagonal HoMnO_{3} single crystals [35]. As shown in Figure 8(a), the amplitude as a function of temperature shows a significant drop to cross zero amplitude line to become negative at some characteristic temperatures. The excitation photon energy used in the experiment changes from 1.52 to 1.68 eV, which is exactly the range covering the d-d transition energy (transition from to ) in the hexagonal ReMnO_{3}. When the photon energy is larger than , the electrons in the orbit can transfer to the unoccupied orbital by absorbing pumping photons. Conversely, this onsite transition would be completely blocked when the transition energy becomes larger than the pumping photon energy. Thus, the amplitude vanishes at a certain temperature , which drops with increasing photon energy, indicating the blueshift of . Furthermore, Shih et al. found that the optical pump-probe measurement is sensitive to short-range magnetic order. In Figure 8(b), the as a function of demonstrates a gradual increase in the extent of antiferromagnetic (AFM) ordering. Moreover, this ordering starts to deviate from linearity around (~76 K), suggesting the prevalence of global long-range AFM ordering. The AFM correlation evolves with temperature as it is close to , shown as in Figure 8(c). Later, Wu et al. obtained similar results for hexagonal YMnO_{3} thin films [74]. Furthermore, they found that the strain-induced changes of , which are difficult to be observed by the temperature-dependent magnetization measurements, can be clearly revealed by the shift of .

As a result, the amplitude of the initial rising component of corresponding to the Mn^{3+} d-d transition is caused by strong coupling between the electronic structure and magnetic ordering. Moreover, the emergence of long-range and short-range magnetic orders can be clearly observed by optical pump-probe spectroscopy.

##### 4.2. Spin-Lattice Coupling

Optically induced lattice vibration can be observed through optical pump-probe spectroscopy through a periodic oscillation. This periodic oscillation in reflectivity (or transmissivity), so-called coherent acoustic phonons, is caused by interference between the reflected probe beams from sample surface and the wave front of the propagating strain pulse generated upon the pump pulse [75, 76]. On the other hand, vibration with frequencies corresponding to optical phonon modes in various materials has been observed by pump-probe spectroscopy. A number of mechanisms have been proposed to explain these oscillations, for example, the displacive excitation of coherent phonons (DECP) [77] and the impulsive stimulated Raman scattering (ISRS) [78, 79]. The simplest idea is that a pump pulse creates a standing wave which was generated by the coherent ionic motion. Then a following probe pulse senses the changes of refractive index which is modulated by the standing wave. In general, the reflectivity (or transmissivity) oscillation observed in pump-probe spectroscopy always corresponds to the optical phonon modes observed in Raman spectroscopy. In conclusion, the measurements of coherent acoustic or optical phonons dynamics at various temperatures are useful to study the spin-lattice coupling in multiferroic materials.

###### 4.2.1. Coherent Optical Phonons

Figure 9 shows the reflectivity oscillation of ~3.6 THz (~120 cm^{−1}) in LuMnO_{3} [36, 37]. According to Raman studies, this vibration mode can be attributed to optical phonon of symmetry [80–82]. This fully symmetric mode corresponds to the Lu1 and Lu2 atomic motions in opposite directions along the *c*-axis, as depicted in Figure 9(d) [36]. In temperature-dependent measurements, the optical phonon almost disappears below , as shown in Figures 9(e) and 9(f) [37]. Additionally, the structural change from highly symmetry space group /mmc to the tilted and distorted *cm* ferroelectric structure [14] in hexagonal manganites (see Figure 1) takes place at the Curie temperature (), which is much higher than . Since there is no structural transition near , the atomic motions of the optical phonon mode would be affected by the appearance of magnetic ordering. In other words, the disappearance of optical phonon mode might be attributed to the magneto-elastic coupling. In temperature-dependent Raman studies, the lowest frequency mode also shows anomaly at in YMnO_{3} [82], ErMnO_{3} [83], and LuMnO_{3} [80, 82] which support close relation between phonon and spin systems.

###### 4.2.2. Coherent Acoustic Phonons

Coherent acoustic phonons have been observed in many kinds of hexagonal manganites such as LuMnO_{3} [37, 84], YMnO_{3} [39], and HoMnO_{3} [38]. The damped oscillation behavior in reflectivity changes with time delay could be described as follows [76]:
where is the wavelength of the probe pulses, is the refraction index of samples without strain, is the strained layer propagating sound speed, and is the penetration depth of probe pulses. The frequency of the oscillation is given as and the dephasing time is .

According to (4), the dephasing time is proportional to the penetration depth of probe pulses and the inverse sound velocity . However, the skin depth is much shorter than the propagating length of the strain pulse. Therefore, the dephasing time is dominated by the finite penetration depth of the probe [84]. The dephasing time of acoustic phonons shows strong temperature dependence (Figure 10), and the anomalous increase of the dephasing time near might be because of the photon energy being close to the edge of d-d transition. In other words, the penetration depth increases and the absorption of probe photons for the d-d transition decreases (due to the blueshift of as mentioned in Section 3.1) as the temperature decreases.

The amplitude and period of the oscillation component in show strong temperature dependence as shown in Figure 11. Both of these parameters are clearly anomalous near the magnetic ordering temperature . The amplitude of the oscillation component in gradually increases with decreasing temperature and reaches the maximum near a characteristic temperature (~190 K for YMnO_{3} [39] and ~200 K for LuMnO_{3} [37]). Then it decreases when the temperature approaches , as shown in Figure 11(a). This may imply the appearance of AFM short-range ordering, as mentioned in [35]. On the other hand, the period of the oscillation component in also slightly shrinks with decreasing temperature. Surprisingly, it dramatically shrinks around as shown in Figure 11(b). This strongly indicates the close correlation between AFM ordering and the propagation of thermal stress along *c*-axis, which is consistent with the results in heat capacity measurements [13, 85]. In addition, the ferroelectric polarization along the *c*-axis caused by polyhedron tilting of MnO_{5} and distortion of the rare-earth ions [14] is well known. Thus, the propagation of a strain pulse with the modulation of dielectric constant (or ferroelectric polarization) along *c*-axis is indeed affected by the appearance of AFM ordering. Neutron diffraction experiments also have demonstrated the extra displacement of the rare-earth and oxygen atoms along *c*-axis at [52]. Finally, these results in amplitude and period of the oscillation component in provide evidence for magnetoelastic coupling in these intriguing materials.

#### 5. Summary and Outlook

In this paper, the recent developments on the electronic structures and ultrafast dynamics of hexagonal manganites have been reviewed. The electronic structure can be clearly revealed by the static linear optical absorption spectra and nonlinear second harmonic generation spectra. The temperature-dependent d-d transition energy exhibits an unexpected change near the spin ordering temperature . This strongly indicates the coupling between electronic structure and antiferromagnetism in hexagonal manganites. Fortunately, the photon energy of the pulse laser used in pump-probe spectroscopy accidentally fits well the d-d transition (from to ) energy. Therefore, the pump-probe measurements can reveal the ultrafast dynamics through the spin-charge coupling and spin-phonon coupling.

However, those ultrafast dynamic experiments only present the charge dynamics between and . If the laser spectrum could cover the whole range of d-d transition, that is, containing the transition from to and to , it could disclose all of the charge dynamics in these strongly magnetic influenced d orbitals. The optical parametric amplifier (OPA) is a suitable light source for this kind of study. Consequently, if all of the charge dynamics in the d orbitals could be completely revealed, it would shed light on the microscopic mechanism of the magnetoelectric coupling or magnetoelastic effect in this kind of strongly correlated material.

#### Acknowledgments

This work was supported by the National Science Council of Taiwan, under Grants nos. NSC98-2112-M-009-008-MY3, NSC101-2112-M-009-016-MY2 and by the MOEATU Program at NCTU of Taiwan, Taiwan.

#### References

- M. Fiebig, “Revival of the magnetoelectric effect,”
*Journal of Physics D*, vol. 38, no. 8, pp. R123–R152, 2005. View at Google Scholar - D. I. Khomskii, “Multiferroics: different ways to combine magnetism and ferroelectricity,”
*Journal of Magnetism and Magnetic Materials*, vol. 306, no. 1, pp. 1–8, 2006. View at Publisher · View at Google Scholar · View at Scopus - W. Eerenstein, N. D. Mathur, and J. F. Scott, “Multiferroic and magnetoelectric materials,”
*Nature*, vol. 442, no. 7104, pp. 759–765, 2006. View at Publisher · View at Google Scholar · View at Scopus - C. W. Nan, M. I. Bichurin, S. Dong, D. Viehland, and G. Srinivasan, “Multiferroic magnetoelectric composites: historical perspective, status, and future directions,”
*Journal of Applied Physics*, vol. 103, no. 3, Article ID 031101, 2008. View at Publisher · View at Google Scholar · View at Scopus - T. Lottermoser, T. Lonkai, U. Amann, D. Hohlwein, J. Ihringer, and M. Fiebig, “Magnetic phase control by an electric field,”
*Nature*, vol. 430, no. 6999, pp. 541–544, 2004. View at Publisher · View at Google Scholar · View at Scopus - B. Lorenz, Y. Q. Wang, and C. W. Chu, “Ferroelectricity in perovskite HoMnO
_{3}and YMnO_{3},”*Physical Review B*, vol. 76, no. 10, Article ID 104405, 2007. View at Publisher · View at Google Scholar · View at Scopus - B. Lorenz, Y. Q. Wang, Y. Y. Sun, and C. W. Chu, “Large magnetodielectric effects in orthorhombic HoMnO
_{3}and YMnO_{3},”*Physical Review B*, vol. 70, no. 21, Article ID 212412, 2004. View at Publisher · View at Google Scholar · View at Scopus - T. Kimura, T. Goto, H. Shintani, K. Ishizaka, T. Arima, and Y. Tokura, “Magnetic control of ferroelectric polarization,”
*Nature*, vol. 426, no. 6962, pp. 55–58, 2003. View at Publisher · View at Google Scholar · View at Scopus - M. Fiebig, T. Lottermoser, D. Fröhlich, A. V. Goltsev, and R. V. Pisarev, “Observation of coupled magnetic and electric domains,”
*Nature*, vol. 419, no. 6909, pp. 818–820, 2002. View at Publisher · View at Google Scholar · View at Scopus - N. Hur, S. Park, P. A. Sharma, J. S. Ahn, S. Guha, and S. W. Cheong, “Electric polarization reversal and memory in a multiferroic material induced by magnetic fields,”
*Nature*, vol. 429, no. 6990, pp. 392–395, 2004. View at Publisher · View at Google Scholar · View at Scopus - W. Prellier, M. P. Singh, and P. Murugavel, “The single-phase multiferroic oxides: from bulk to thin film,”
*Journal of Physics*, vol. 17, no. 30, pp. R803–R832, 2005. View at Publisher · View at Google Scholar · View at Scopus - S. W. Cheong and M. Mostovoy, “Multiferroics: a magnetic twist for ferroelectricity,”
*Nature Materials*, vol. 6, no. 1, pp. 13–20, 2007. View at Publisher · View at Google Scholar · View at Scopus - T. Katsufuji, S. Mori, M. Masaki, Y. Moritomo, N. Yamamoto, and H. Takagi, “Dielectric and magnetic anomalies and spin frustration in hexagonal
*R*MnO_{3}(*R*= Y, Yb, and Lu),”*Physical Review B*, vol. 64, no. 10, Article ID 104419, 2001. View at Google Scholar · View at Scopus - B. B. Van Aken, T. T. M. Palstra, A. Filippetti, and N. A. Spaldin, “The origin of ferroelectricity in magnetoelectric YMnO
_{3},”*Nature Materials*, vol. 3, no. 3, pp. 164–170, 2004. View at Google Scholar · View at Scopus - C. J. Fennie and K. M. Rabe, “Ferroelectric transition in YMnO
_{3}from first principles,”*Physical Review B*, vol. 72, no. 10, Article ID 100103, 2005. View at Publisher · View at Google Scholar · View at Scopus - T. H. Lin, C. C. Hsieh, H. C. Shih et al., “Anomalous magnetic ordering in
*b*-axis-oriented orthorhombic HoMnO_{3}thin films,”*Applied Physics Letters*, vol. 92, no. 13, Article ID 132503, 2008. View at Publisher · View at Google Scholar · View at Scopus - M. N. Iliev, M. V. Abrashev, H. G. Lee et al., “Raman spectroscopy of orthorhombic perovskitelike YMnO
_{3}and LaMnO_{3},”*Physical Review B*, vol. 57, no. 5, pp. 2872–2877, 1998. View at Google Scholar · View at Scopus - J. S. Zhou and J. B. Goodenough, “Unusual evolution of the magnetic interactions versus structural distortions in
*R*MnO_{3}perovskites,”*Physical Review Letters*, vol. 96, no. 24, Article ID 247202, 2006. View at Publisher · View at Google Scholar · View at Scopus - W. C. Yi, C. S. Seo, S. I. Kwun, and J. G. Yoon, “Temperature dependence of capacitance/current-voltage characteristics of highly (0001)-oriented YMnO
_{3}thin films on Si,”*Applied Physics Letters*, vol. 77, no. 7, pp. 1044–1046, 2000. View at Google Scholar · View at Scopus - H. N. Lee, Y. T. Kim, and S. H. Choh, “Comparison of memory effect between YMnO
_{3}and SrBi_{2}Ta_{2}O_{9}ferroelectric thin films deposited on Si substrates,”*Applied Physics Letters*, vol. 76, no. 8, pp. 1066–1068, 2000. View at Google Scholar · View at Scopus - S. Imada, T. Kuraoka, E. Tokumitsu, and H. Ishiwara, “Ferroelectricity of YMnO
_{3}thin films on Pt(111)/Al_{2}O_{3}(0001) and Pt(111)/Y_{2}O_{3}(111)/Si(111) structures grown by molecular beam epitaxy,”*Japanese Journal of Applied Physics*, vol. 40, no. 2 A, pp. 666–671, 2001. View at Google Scholar · View at Scopus - Y. T. Kim, I. S. Kim, S. I. Kim, D. C. Yoo, and J. Y. Lee, “Atomic structure of random and
*c*-axis oriented YMnO_{3}thin films deposited on Si and Y_{2}O_{3}/Si substrates,”*Journal of Applied Physics*, vol. 94, no. 8, pp. 4859–4862, 2003. View at Publisher · View at Google Scholar · View at Scopus - T. Yoshimura, N. Fujimura, and T. Ito, “Ferroelectric properties of
*c*-oriented YMnO_{3}films deposited on Si substrates,”*Applied Physics Letters*, vol. 73, no. 3, pp. 414–416, 1998. View at Publisher · View at Google Scholar · View at Scopus - T. Lonkai, D. G. Tomuta, U. Amann et al., “Development of the high-temperature phase of hexagonal manganites,”
*Physical Review B*, vol. 69, no. 13, Article ID 134108, 2004. View at Publisher · View at Google Scholar · View at Scopus - N. Fujimura, T. Ishida, T. Yoshimura, and T. Ito, “Epitaxially grown YMnO
_{3}film: new candidate for nonvolatile memory devices,”*Applied Physics Letters*, vol. 69, no. 7, pp. 1011–1013, 1996. View at Google Scholar · View at Scopus - T. Kimura, S. Ishihara, H. Shintani et al., “Distorted perovskite with eg1 configuration as a frustrated spin system,”
*Physical Review B*, vol. 68, no. 6, Article ID 060403, 2003. View at Google Scholar · View at Scopus - T. Goto, T. Kimura, G. Lawes, A. P. Ramirez, and Y. Tokura, “Ferroelectricity and giant magnetocapacitance in perovskite rare-earth manganites,”
*Physical Review Letters*, vol. 92, no. 25, Article ID 257201, 2004. View at Publisher · View at Google Scholar · View at Scopus - M. Tachibana, T. Shimoyama, H. Kawaji, T. Atake, and E. Takayama-Muromachi, “Jahn-Teller distortion and magnetic transitions in perovskite
*R*MnO_{3}(*R*= Ho, Er, Tm, Yb, and Lu),”*Physical Review B*, vol. 75, no. 14, Article ID 14425, 2007. View at Google Scholar - N. Iwata and K. Kohn, “Dielectric anomalies at magnetic transitions of hexagonal rare earth manganese oxides
*R*MnO_{3},”*Journal of the Physical Society of Japan*, vol. 67, no. 9, pp. 3318–3319, 1998. View at Google Scholar · View at Scopus - J. E. Medvedeva, V. I. Anisimov, M. A. Korotin, O. N. Mryasov, and A. J. Freeman, “Effect of Coulomb correlation and magnetic ordering on the electronic structure of two hexagonal phases of ferroelectromagnetic YMnO
_{3},”*Journal of Physics Condensed Matter*, vol. 12, no. 23, pp. 4947–4958, 2000. View at Publisher · View at Google Scholar · View at Scopus - A. B. Souchkov, J. R. Simpson, M. Quijada et al., “Exchange interaction effects on the optical properties of LuMnO
_{3},”*Physical Review Letters*, vol. 91, no. 2, Article ID 027203, 2003. View at Google Scholar · View at Scopus - W. S. Choi, S. J. Moon, S. S. A. Seo et al., “Optical spectroscopic investigation on the coupling of electronic and magnetic structure in multiferroic hexagonal
*R*MnO_{3}(*R*= Gd, Tb, Dy, and Ho) thin films,”*Physical Review B*, vol. 78, no. 5, Article ID 054440, 2008. View at Publisher · View at Google Scholar · View at Scopus - M. Fiebig, D. Fröhlich, K. Kohn et al., “Determination of the magnetic symmetry of hexagonal manganites by second harmonic generation,”
*Physical Review Letters*, vol. 84, no. 24, pp. 5620–5623, 2000. View at Publisher · View at Google Scholar · View at Scopus - D. Fröhlich, S. Leute, V. V. Pavlov, and R. V. Pisarev, “Nonlinear optical spectroscopy of the two-order-parameter compound YMnO
_{3},”*Physical Review Letters*, vol. 81, no. 15, pp. 3239–3242, 1998. View at Google Scholar · View at Scopus - H. C. Shih, T. H. Lin, C. W. Luo et al., “Magnetization dynamics and the Mn
^{3+}*d-d*excitation of hexagonal HoMnO_{3}single crystals using wavelength-tunable time-resolved femtosecond spectroscopy,”*Physical Review B*, vol. 80, no. 2, Article ID 024427, 2009. View at Publisher · View at Google Scholar · View at Scopus - S. T. Lou, F. M. Zimmermann, R. A. Bartynski, N. Hur, and S. W. Cheong, “Femtosecond laser excitation of coherent optical phonons in ferroelectric LuMnO
_{3},”*Physical Review B*, vol. 79, no. 21, Article ID 214301, 2009. View at Publisher · View at Google Scholar · View at Scopus - K. J. Jang, J. Lim, J. Ahn et al., “Ultrafast IR spectroscopic study of coherent phonons and dynamic spin-lattice coupling in multiferroic LuMnO
_{3},”*New Journal of Physics*, vol. 12, no. 2, Article ID 023017, 2010. View at Publisher · View at Google Scholar · View at Scopus - H. C. Shih, L. Y. Chen, C. W. Luo et al., “Ultrafast thermoelastic dynamics of HoMnO
_{3}single crystals derived from femtosecond optical pump-probe spectroscopy,”*New Journal of Physics*, vol. 13, no. 5, Article ID 053003, 2011. View at Publisher · View at Google Scholar · View at Scopus - K. J. Jang, H. G. Lee, S. Lee et al., “Strong spin-lattice coupling in multiferroic hexagonal manganite YMnO
_{3}probed by ultrafast optical spectroscopy,”*Applied Physics Letters*, vol. 97, no. 3, Article ID 031914, 2010. View at Publisher · View at Google Scholar · View at Scopus - B. G. Ueland, J. W. Lynn, M. Laver, Y. J. Choi, and S. W. Cheong, “Origin of electric-field-induced magnetization in multiferroic HoMnO
_{3},”*Physical Review Letters*, vol. 104, no. 14, Article ID 147204, 2010. View at Publisher · View at Google Scholar · View at Scopus - M. Fiebig, C. Degenhardt, and R. V. Pisarev, “Interaction of frustrated magnetic sublattices in ErMnO
_{3},”*Physical Review Letters*, vol. 88, no. 2, Article ID 027203, 2002. View at Publisher · View at Google Scholar · View at Scopus - O. P. Vajk, M. Kenzelmann, J. W. Lynn, S. B. Kim, and S. W. Cheong, “Magnetic order and spin dynamics in ferroelectric HoMnO
_{3},”*Physical Review Letters*, vol. 94, no. 8, Article ID 087601, 2005. View at Publisher · View at Google Scholar · View at Scopus - H. Lueken, “A magnetoelectric effect in YMnO
_{3}and HoMnO_{3},”*Angewandte Chemie*, vol. 47, no. 45, pp. 8562–8564, 2008. View at Publisher · View at Google Scholar · View at Scopus - D. Khomskii, “Classifying multiferroics: mechanisms and effects,”
*Physics*, vol. 2 , article 20, 2009. View at Publisher · View at Google Scholar - A. Muñoz, J. A. Alonso, M. J. Martínez-Lope, M. T. Casáis, J. L. Martínez, and M. T. Fernández-Díaz, “Magnetic structure of hexagonal
*R*MnO_{3}(*R*= Y, Sc): thermal evolution from neutron powder diffraction data,”*Physical Review B*, vol. 62, no. 14, pp. 9498–9510, 2000. View at Google Scholar - A. Muñoz, J. A. Alonso, M. J. Martínez-Lope, M. T. Casáis, J. L. Martínez, and M. T. Fernández-Díaz, “Evolution of the magnetic structure of hexagonal HoMnO
_{3}from neutron powder diffraction data,”*Chemistry of Materials*, vol. 13, no. 5, pp. 1497–1505, 2001. View at Google Scholar - M. Fiebig, C. Degenhardt, and R. V. Pisarev, “Magnetic phase diagram of HoMnO
_{3},”*Journal of Applied Physics*, vol. 91, no. 10, pp. 8867–8869, 2002. View at Publisher · View at Google Scholar · View at Scopus - T. Lonkai, D. G. Tomuta, J. U. Hoffmann, R. Schneider, D. Hohlwein, and J. Ihringer, “Magnetic two-dimensional short-range order in hexagonal manganites,”
*Journal of Applied Physics*, vol. 93, no. 10, pp. 8191–8193, 2003. View at Publisher · View at Google Scholar · View at Scopus - Z. J. Huang, Y. Cao, Y. Y. Sun, Y. Y. Xue, and C. W. Chu, “Coupling between the ferroelectric and antiferromagnetic orders in YMnO
_{3},”*Physical Review B*, vol. 56, no. 5, pp. 2623–2626, 1997. View at Google Scholar · View at Scopus - D. G. Tomuta, S. Ramakrishnan, G. J. Niewenhuys, and J. A. Mydosh, “The magnetic susceptibility, specific heat and dielectric constant of hexagonal YMnO
_{3}, LuMnO_{3}and ScMnO_{3},”*Journal of Physics Condensed Matter*, vol. 13, no. 20, pp. 4543–4552, 2001. View at Publisher · View at Google Scholar · View at Scopus - C. Dela Cruz, F. Yen, B. Lorenz et al., “Strong spin-lattice coupling in multiferroic HoMnO
_{3}: thermal expansion anomalies and pressure effect,”*Physical Review B*, vol. 71, no. 6, Article ID 060407(R), 2005. View at Publisher · View at Google Scholar · View at Scopus - S. Lee, A. Pirogov, M. Kang et al., “Giant magneto-elastic coupling in multiferroic hexagonal manganites,”
*Nature*, vol. 451, no. 7180, pp. 805–809, 2008. View at Google Scholar - D. Y. Cho, J. Y. Kim, B. G. Park et al., “Ferroelectricity driven by y d0-ness with rehybridization in YMnO
_{3},”*Physical Review Letters*, vol. 98, no. 21, Article ID 217601, 2007. View at Publisher · View at Google Scholar · View at Scopus - D. Talbayev, S. A. Trugman, A. V. Balatsky, T. Kimura, A. J. Taylor, and R. D. Averitt, “Detection of coherent magnons via ultrafast pump-probe reflectance spectroscopy in multiferroic Ba
_{0.6}Sr_{1.4}Zn_{2}Fe_{12}O_{22},”*Physical Review Letters*, vol. 101, no. 9, Article ID 097603, 2008. View at Publisher · View at Google Scholar · View at Scopus - A. V. Kimel, B. A. Ivanov, R. V. Pisarev, P. A. Usachev, A. Kirilyuk, and T. Rasing, “Inertia-driven spin switching in antiferromagnets,”
*Nature Physics*, vol. 5, no. 10, pp. 727–731, 2009. View at Publisher · View at Google Scholar · View at Scopus - C. W. Luo, I. H. Wu, P. C. Cheng et al., “Quasiparticle dynamics and phonon softening in FeSe superconductors,”
*Physical Review Letters*, vol. 108, no. 25, Article ID 257006, 2012. View at Google Scholar - C. W. Luo, I. H. Wu, P. C. Cheng et al., “Ultrafast dynamics and phonon softening in Fe
_{1+y}Se_{1−x}Te_{x}single crystals,”*New Journal of Physics*, vol. 14, no. 10, Article ID 103053, 2012. View at Google Scholar - A. V. Kimel, R. V. Pisarev, F. Bentivegna, and T. Rasing, “Time-resolved nonlinear optical spectroscopy of Mn
^{3+}ions in rare-earth hexagonal manganites*R*MnO_{3}(*R*= Sc, Y, Er),”*Physical Review B*, vol. 64, no. 20, Article ID 201103(R), 2001. View at Google Scholar · View at Scopus - A. V. Kimel, R. V. Pisarev, F. Bentivegna, and Th. Rasing, “Ultrafast optical spectroscopy of hexagonal manganites
*R*MnO_{3}(*R*= Y, Er, Sc),”*Ferroelectrics*, vol. 279, no. 1, pp. 135–176, 2002. View at Google Scholar - W. C. Yi, S. I. Kwun, and J. G. Yoon, “Study on the electronic structure of hexagonal and orthorhombic YMnO
_{3},”*Journal of the Physical Society of Japan*, vol. 69, no. 8, pp. 2706–2707, 2000. View at Google Scholar · View at Scopus - A. Filippetti and N. A. Hill, “Coexistence of magnetism and ferroelectricity in perovskites,”
*Physical Review B*, vol. 65, no. 19, Article ID 195120, 2002. View at Google Scholar - K. Kritayakirana, P. Berger, and R. V. Jones, “Optical spectra of ferroelectric-antiferromagnetic rare earth manganates,”
*Optics Communications*, vol. 1, no. 3, pp. 95–98, 1969. View at Google Scholar · View at Scopus - A. M. Kalashnikova and R. V. Pisarev, “Electronic structure of hexagonal rare-earth manganites
*R*MnO_{3},”*JETP Letters*, vol. 78, no. 3, pp. 143–147, 2003. View at Publisher · View at Google Scholar · View at Scopus - R. C. Rai, J. Cao, J. L. Musfeldt, S. B. Kim, S. W. Cheong, and X. Wei, “Spin-charge coupling and the high-energy magnetodielectric effect in hexagonal HoMnO
_{3},”*Physical Review B*, vol. 75, no. 18, Article ID 184414, 2007. View at Publisher · View at Google Scholar · View at Scopus - J. S. Kang, S. W. Han, J. G. Park et al., “Photoemission and x-ray absorption of the electronic structure of multifferroic
*R*MnO_{3}(*R*= Y, Er),”*Physical Review B*, vol. 71, no. 9, Article ID 092405, 2005. View at Google Scholar - M. Qian, J. Dong, and D. Y. Xing, “Optical properties of the ferroelectromagnet YMnO
_{3}studied from first principles,”*Physical Review B*, vol. 63, no. 15, Article ID 155101, 2001. View at Google Scholar · View at Scopus - W. S. Choi, D. G. Kim, S. S. A. Seo et al., “Electronic structures of hexagonal
*R*MnO_{3}(*R*= Gd, Tb, Dy, and Ho) thin films: optical spectroscopy and first-principles calculations,”*Physical Review B*, vol. 77, no. 4, Article ID 045137, 2008. View at Publisher · View at Google Scholar · View at Scopus - M. Fiebig, V. V. Pavlov, and R. V. Pisarev, “Second-harmonic generation as a tool for studying electronic and magnetic structures of crystals: review,”
*Journal of the Optical Society of America B*, vol. 22, no. 1, pp. 96–118, 2005. View at Publisher · View at Google Scholar · View at Scopus - C. Degenhardt, M. Fiebig, D. Fröhlich, T. Lottermoser, and R. V. Pisarev, “Nonlinear optical spectroscopy of electronic transitions in hexagonal manganites,”
*Applied Physics B*, vol. 73, no. 2, pp. 139–144, 2001. View at Google Scholar · View at Scopus - V. M. Axt and T. Kuhn, “Femtosecond spectroscopy in semiconductors: a key to coherences, correlations and quantum kinetics,”
*Reports on Progress in Physics*, vol. 67, no. 4, pp. 433–512, 2004. View at Publisher · View at Google Scholar · View at Scopus - S. K. Sundaram and E. Mazur, “Inducing and probing non-thermal transitions in semiconductors using femtosecond laser pulses,”
*Nature Materials*, vol. 1, no. 4, pp. 217–224, 2002. View at Publisher · View at Google Scholar · View at Scopus - R. D. Averitt and A. J. Taylor, “Ultrafast optical and far-infrared quasiparticle dynamics in correlated electron materials,”
*Journal of Physics Condensed Matter*, vol. 14, no. 50, pp. R1357–R1390, 2002. View at Publisher · View at Google Scholar · View at Scopus - C. W. Luo, Y. T. Wang, F. W. Chen et al., “Eliminate coherence spike in reflection-type pump-probe measurements,”
*Optics Express*, vol. 17, no. 14, pp. 11321–11327, 2009. View at Google Scholar - K. H. Wu, H. J. Chen, Y. T. Chen et al., “Marked enhancement of Néel temperature in strained YMnO
_{3}thin films probed by femtosecond spectroscopy,”*Europhysics Letters*, vol. 94, no. 2, Article ID 27006, 2011. View at Publisher · View at Google Scholar · View at Scopus - C. Thomsen, J. Strait, Z. Vardeny, H. J. Maris, J. Tauc, and J. J. Hauser, “Coherent phonon generation and detection by picosecond light pulses,”
*Physical Review Letters*, vol. 53, no. 10, pp. 989–992, 1984. View at Publisher · View at Google Scholar · View at Scopus - C. Thomsen, H. T. Grahn, H. J. Maris, and J. Tauc, “Surface generation and detection of phonons by picosecond light pulses,”
*Physical Review B*, vol. 34, no. 6, pp. 4129–4138, 1986. View at Publisher · View at Google Scholar · View at Scopus - H. J. Zeiger, J. Vidal, T. K. Cheng, E. P. Ippen, G. Dresselhaus, and M. S. Dresselhaus, “Theory for displacive excitation of coherent phonons,”
*Physical Review B*, vol. 45, no. 2, pp. 768–778, 1992. View at Publisher · View at Google Scholar · View at Scopus - R. Merlin, “Generating coherent THz phonons with light pulses,”
*Solid State Communications*, vol. 102, no. 2-3, pp. 207–220, 1997. View at Google Scholar - G. A. Garrett, T. F. Albrecht, J. F. Whitaker, and R. Merlin, “Coherent THz phonons driven by light pulses and the Sb problem: what is the mechanism?”
*Physical Review Letters*, vol. 77, no. 17, pp. 3661–3664, 1996. View at Google Scholar · View at Scopus - A. Ghosh, J. R. Sahu, S. V. Bhat, and C. N. R. Rao, “A Raman study of multiferroic LuMnO
_{3},”*Solid State Sciences*, vol. 11, no. 9, pp. 1639–1642, 2009. View at Publisher · View at Google Scholar · View at Scopus - A. P. Litvinchuk, M. N. Iliev, V. N. Popov, and M. M. Gospodinov, “Raman and infrared-active phonons in hexagonal HoMnO
_{3}single crystals: magnetic ordering effects,”*Journal of Physics Condensed Matter*, vol. 16, no. 6, pp. 809–819, 2004. View at Publisher · View at Google Scholar · View at Scopus - J. Vermette, S. Jandl, A. A. Mukhin et al., “Raman study of the antiferromagnetic phase transitions in hexagonal YMnO
_{3}and LuMnO_{3},”*Journal of Physics Condensed Matter*, vol. 22, no. 35, Article ID 356002, 2010. View at Publisher · View at Google Scholar · View at Scopus - J. Vermette, S. Jandl, and M. M. Gospodinov, “Raman study of spin-phonon coupling in ErMnO
_{3},”*Journal of Physics*, vol. 20, no. 42, Article ID 425219, 2008. View at Google Scholar - D. Lim, R. D. Averitt, J. Demsar, A. J. Taylor, N. Hur, and S. W. Cheong, “Coherent acoustic phonons in hexagonal manganite LuMnO
_{3},”*Applied Physics Letters*, vol. 83, no. 23, pp. 4800–4802, 2003. View at Publisher · View at Google Scholar · View at Scopus - P. A. Sharma, J. S. Ahn, N. Hur et al., “Thermal conductivity of geometrically frustrated, ferroelectric YMnO
_{3}: extraordinary spin-phonon interactions,”*Physical Review Letters*, vol. 93, no. 17, Article ID 177202, p. 1, 2004. View at Publisher · View at Google Scholar · View at Scopus